#------------------------------------------------------------------------------
#$Date: 2019-11-17 05:03:17 +0200 (Sun, 17 Nov 2019) $
#$Revision: 228016 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/12/17/7121799.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7121799
loop_
_publ_author_name
'Ovchinnikov, Alexander'
'Makongo, Julien P. A.'
'Bobev, Svilen'
_publ_section_title
;
 Yet again, new compounds found in systems with known binary phase
 diagrams. Synthesis, crystal and electronic structure of
 Nd₃Bi₇ and Sm₃Bi₇.
;
_journal_issue                   51
_journal_name_full
'Chemical communications (Cambridge, England)'
_journal_page_first              7089
_journal_page_last               7092
_journal_paper_doi               10.1039/c8cc02563k
_journal_volume                  54
_journal_year                    2018
_chemical_formula_sum            'Bi7 Nd3'
_chemical_formula_weight         1895.58
_space_group_crystal_system      orthorhombic
_space_group_IT_number           71
_space_group_name_Hall           '-I 2 2'
_space_group_name_H-M_alt        'I m m m'
_symmetry_space_group_name_Hall  '-I 2 2'
_symmetry_space_group_name_H-M   'I m m m'
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2018-03-27 deposited with the CCDC.
2018-06-04 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.2996(6)
_cell_length_b                   15.200(2)
_cell_length_c                   19.121(3)
_cell_measurement_reflns_used    578
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      29.73
_cell_measurement_theta_min      5.14
_cell_volume                     1249.6(3)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0748
_diffrn_reflns_av_unetI/netI     0.0658
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            5960
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.740
_diffrn_reflns_theta_min         1.711
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    110.339
_exptl_absorpt_correction_T_max  0.051
_exptl_absorpt_correction_T_min  0.010
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    10.076
_exptl_crystal_description       block
_exptl_crystal_F_000             3044
_exptl_crystal_size_max          0.070
_exptl_crystal_size_mid          0.060
_exptl_crystal_size_min          0.040
_refine_diff_density_max         3.213
_refine_diff_density_min         -3.895
_refine_diff_density_rms         0.787
_refine_ls_extinction_coef       0.00025(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.021
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     38
_refine_ls_number_reflns         1159
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.021
_refine_ls_R_factor_all          0.0555
_refine_ls_R_factor_gt           0.0399
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0248P)²] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0824
_refine_ls_wR_factor_ref         0.0893
_reflns_Friedel_coverage         0.000
_reflns_number_gt                882
_reflns_number_total             1159
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c8cc02563k2.cif
_cod_data_source_block           shelx
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 

 Adding full bibliography for 7121799--7121800.cif.
;
_cod_database_code               7121799
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.048
_shelx_estimated_absorpt_t_max   0.096
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'x, -y, -z'
'-x, y, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'-x, y, z'
'x, -y, z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'-x+1/2, y+1/2, z+1/2'
'x+1/2, -y+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Nd1 Nd 0.0000 0.13913(7) 0.36829(6) 0.0158(2) Uani 1 2 d S T P
Nd2 Nd 0.0000 0.0000 0.17266(8) 0.0160(3) Uani 1 4 d S T P
Bi1 Bi 0.0000 0.21176(5) 0.19682(4) 0.01695(19) Uani 1 2 d S T P
Bi2 Bi 0.0000 0.36019(5) 0.41198(4) 0.0190(2) Uani 1 2 d S T P
Bi3 Bi 0.5000 0.0000 0.30090(6) 0.0164(2) Uani 1 4 d S T P
Bi4 Bi 0.0000 0.33521(7) 0.0000 0.0179(2) Uani 1 4 d S T P
Bi5 Bi 0.5000 0.5000 0.0000 0.0191(3) Uani 1 8 d S T P
Bi6 Bi 0.0000 0.0000 0.0000 0.0213(3) Uani 1 8 d S T P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nd Nd -0.1943 3.0179 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Bi3 Nd1 Bi3 81.93(3) . 1_455
Bi3 Nd1 Bi5 83.46(3) . 5_445
Bi3 Nd1 Bi5 83.47(3) 1_455 5_445
Bi3 Nd1 Bi4 87.11(2) . 13
Bi3 Nd1 Bi4 142.65(4) 1_455 13
Bi5 Nd1 Bi4 59.79(2) 5_445 13
Bi3 Nd1 Bi4 142.65(4) . 13_455
Bi3 Nd1 Bi4 87.11(2) 1_455 13_455
Bi5 Nd1 Bi4 59.79(2) 5_445 13_455
Bi4 Nd1 Bi4 80.30(3) 13 13_455
Bi3 Nd1 Bi1 82.54(2) . 13
Bi3 Nd1 Bi1 135.10(4) 1_455 13
Bi5 Nd1 Bi1 135.80(2) 5_445 13
Bi4 Nd1 Bi1 77.79(2) 13 13
Bi4 Nd1 Bi1 127.80(4) 13_455 13
Bi3 Nd1 Bi1 135.10(4) . 13_455
Bi3 Nd1 Bi1 82.54(2) 1_455 13_455
Bi5 Nd1 Bi1 135.80(2) 5_445 13_455
Bi4 Nd1 Bi1 127.80(4) 13 13_455
Bi4 Nd1 Bi1 77.79(2) 13_455 13_455
Bi1 Nd1 Bi1 79.48(3) 13 13_455
Bi3 Nd1 Bi1 80.41(3) . .
Bi3 Nd1 Bi1 80.41(3) 1_455 .
Bi5 Nd1 Bi1 158.59(4) 5_445 .
Bi4 Nd1 Bi1 132.73(2) 13 .
Bi4 Nd1 Bi1 132.73(2) 13_455 .
Bi1 Nd1 Bi1 55.53(2) 13 .
Bi1 Nd1 Bi1 55.53(2) 13_455 .
Bi3 Nd1 Bi2 136.106(17) . .
Bi3 Nd1 Bi2 136.106(17) 1_455 .
Bi5 Nd1 Bi2 116.06(4) 5_445 .
Bi4 Nd1 Bi2 72.79(3) 13 .
Bi4 Nd1 Bi2 72.79(3) 13_455 .
Bi1 Nd1 Bi2 55.61(2) 13 .
Bi1 Nd1 Bi2 55.61(2) 13_455 .
Bi1 Nd1 Bi2 85.35(3) . .
Bi1 Nd2 Bi1 163.67(6) . 2
Bi1 Nd2 Bi3 83.87(2) . 1_455
Bi1 Nd2 Bi3 83.87(2) 2 1_455
Bi1 Nd2 Bi3 83.87(2) . .
Bi1 Nd2 Bi3 83.87(2) 2 .
Bi3 Nd2 Bi3 82.48(5) 1_455 .
Bi1 Nd2 Bi6 98.17(3) . .
Bi1 Nd2 Bi6 98.17(3) 2 .
Bi3 Nd2 Bi6 138.76(2) 1_455 .
Bi3 Nd2 Bi6 138.76(2) . .
Bi1 Nd2 Bi2 132.89(2) . 14_445
Bi1 Nd2 Bi2 56.876(17) 2 14_445
Bi3 Nd2 Bi2 86.650(18) 1_455 14_445
Bi3 Nd2 Bi2 140.20(2) . 14_445
Bi6 Nd2 Bi2 61.84(3) . 14_445
Bi1 Nd2 Bi2 56.876(17) . 13
Bi1 Nd2 Bi2 132.89(2) 2 13
Bi3 Nd2 Bi2 140.20(2) 1_455 13
Bi3 Nd2 Bi2 86.651(18) . 13
Bi6 Nd2 Bi2 61.84(3) . 13
Bi2 Nd2 Bi2 123.67(5) 14_445 13
Bi1 Nd2 Bi2 56.876(17) . 13_455
Bi1 Nd2 Bi2 132.89(2) 2 13_455
Bi3 Nd2 Bi2 86.650(18) 1_455 13_455
Bi3 Nd2 Bi2 140.20(2) . 13_455
Bi6 Nd2 Bi2 61.84(3) . 13_455
Bi2 Nd2 Bi2 76.60(3) 14_445 13_455
Bi2 Nd2 Bi2 77.66(3) 13 13_455
Bi1 Nd2 Bi2 132.89(2) . 14_545
Bi1 Nd2 Bi2 56.876(17) 2 14_545
Bi3 Nd2 Bi2 140.20(2) 1_455 14_545
Bi3 Nd2 Bi2 86.651(18) . 14_545
Bi6 Nd2 Bi2 61.84(3) . 14_545
Bi2 Nd2 Bi2 77.66(3) 14_445 14_545
Bi2 Nd2 Bi2 76.60(3) 13 14_545
Bi2 Nd2 Bi2 123.67(5) 13_455 14_545
Bi1 Bi1 Bi1 85.09(4) 13 13_455
Bi1 Bi1 Bi2 178.51(4) 13 13_455
Bi1 Bi1 Bi2 94.988(17) 13_455 13_455
Bi1 Bi1 Bi2 94.988(17) 13 13
Bi1 Bi1 Bi2 178.51(4) 13_455 13
Bi2 Bi1 Bi2 84.90(3) 13_455 13
Bi1 Bi1 Nd2 116.92(3) 13 .
Bi1 Bi1 Nd2 116.92(3) 13_455 .
Bi2 Bi1 Nd2 64.36(3) 13_455 .
Bi2 Bi1 Nd2 64.36(3) 13 .
Bi1 Bi1 Nd1 63.78(3) 13 13
Bi1 Bi1 Nd1 115.00(4) 13_455 13
Bi2 Bi1 Nd1 114.91(3) 13_455 13
Bi2 Bi1 Nd1 63.78(2) 13 13
Nd2 Bi1 Nd1 127.92(3) . 13
Bi1 Bi1 Nd1 115.00(4) 13 13_455
Bi1 Bi1 Nd1 63.78(3) 13_455 13_455
Bi2 Bi1 Nd1 63.78(2) 13_455 13_455
Bi2 Bi1 Nd1 114.91(3) 13 13_455
Nd2 Bi1 Nd1 127.92(3) . 13_455
Nd1 Bi1 Nd1 79.48(3) 13 13_455
Bi1 Bi1 Nd1 60.69(3) 13 .
Bi1 Bi1 Nd1 60.69(3) 13_455 .
Bi2 Bi1 Nd1 120.62(3) 13_455 .
Bi2 Bi1 Nd1 120.62(3) 13 .
Nd2 Bi1 Nd1 79.56(4) . .
Nd1 Bi1 Nd1 124.47(2) 13 .
Nd1 Bi1 Nd1 124.47(2) 13_455 .
Bi1 Bi2 Bi1 84.90(3) 13_455 13
Bi1 Bi2 Bi2 130.776(17) 13_455 10_556
Bi1 Bi2 Bi2 130.776(18) 13 10_556
Bi1 Bi2 Nd2 109.13(4) 13_455 13
Bi1 Bi2 Nd2 58.76(2) 13 13
Bi2 Bi2 Nd2 118.17(3) 10_556 13
Bi1 Bi2 Nd2 58.76(2) 13_455 13_455
Bi1 Bi2 Nd2 109.13(4) 13 13_455
Bi2 Bi2 Nd2 118.17(3) 10_556 13_455
Nd2 Bi2 Nd2 77.66(3) 13 13_455
Bi1 Bi2 Bi6 161.44(3) 13_455 5
Bi1 Bi2 Bi6 96.270(14) 13 5
Bi2 Bi2 Bi6 60.894(14) 10_556 5
Nd2 Bi2 Bi6 57.27(3) 13 5
Nd2 Bi2 Bi6 103.80(2) 13_455 5
Bi1 Bi2 Bi6 96.270(14) 13_455 5_455
Bi1 Bi2 Bi6 161.44(3) 13 5_455
Bi2 Bi2 Bi6 60.894(13) 10_556 5_455
Nd2 Bi2 Bi6 103.80(2) 13 5_455
Nd2 Bi2 Bi6 57.27(3) 13_455 5_455
Bi6 Bi2 Bi6 76.833(19) 5 5_455
Bi1 Bi2 Nd1 60.61(2) 13_455 .
Bi1 Bi2 Nd1 60.61(2) 13 .
Bi2 Bi2 Nd1 103.96(2) 10_556 .
Nd2 Bi2 Nd1 119.18(3) 13 .
Nd2 Bi2 Nd1 119.18(3) 13_455 .
Bi6 Bi2 Nd1 135.516(17) 5 .
Bi6 Bi2 Nd1 135.516(17) 5_455 .
Nd2 Bi3 Nd2 82.48(5) 1_655 .
Nd2 Bi3 Nd1 136.69(3) 1_655 .
Nd2 Bi3 Nd1 82.14(2) . .
Nd2 Bi3 Nd1 82.14(2) 1_655 1_655
Nd2 Bi3 Nd1 136.69(3) . 1_655
Nd1 Bi3 Nd1 81.93(3) . 1_655
Nd2 Bi3 Nd1 136.69(3) 1_655 2
Nd2 Bi3 Nd1 82.14(2) . 2
Nd1 Bi3 Nd1 80.31(3) . 2
Nd1 Bi3 Nd1 133.73(5) 1_655 2
Nd2 Bi3 Nd1 82.14(2) 1_655 2_655
Nd2 Bi3 Nd1 136.69(3) . 2_655
Nd1 Bi3 Nd1 133.73(5) . 2_655
Nd1 Bi3 Nd1 80.31(3) 1_655 2_655
Nd1 Bi3 Nd1 81.93(3) 2 2_655
Bi5 Bi4 Bi5 81.28(3) . 1_455
Bi5 Bi4 Nd1 59.422(19) . 13
Bi5 Bi4 Nd1 109.34(3) 1_455 13
Bi5 Bi4 Nd1 109.34(3) . 6_454
Bi5 Bi4 Nd1 59.422(19) 1_455 6_454
Nd1 Bi4 Nd1 166.56(5) 13 6_454
Bi5 Bi4 Nd1 109.34(3) . 13_455
Bi5 Bi4 Nd1 59.422(19) 1_455 13_455
Nd1 Bi4 Nd1 80.30(3) 13 13_455
Nd1 Bi4 Nd1 98.11(3) 6_454 13_455
Bi5 Bi4 Nd1 59.422(19) . 6_554
Bi5 Bi4 Nd1 109.34(3) 1_455 6_554
Nd1 Bi4 Nd1 98.11(3) 13 6_554
Nd1 Bi4 Nd1 80.30(3) 6_454 6_554
Nd1 Bi4 Nd1 166.56(5) 13_455 6_554
Nd1 Bi5 Nd1 180.00(3) 14 6_554
Nd1 Bi5 Nd1 99.96(4) 14 5_554
Nd1 Bi5 Nd1 80.04(4) 6_554 5_554
Nd1 Bi5 Nd1 80.04(4) 14 13
Nd1 Bi5 Nd1 99.96(4) 6_554 13
Nd1 Bi5 Nd1 180.00(4) 5_554 13
Nd1 Bi5 Bi4 60.793(15) 14 9_665
Nd1 Bi5 Bi4 119.207(15) 6_554 9_665
Nd1 Bi5 Bi4 60.793(15) 5_554 9_665
Nd1 Bi5 Bi4 119.207(15) 13 9_665
Nd1 Bi5 Bi4 60.793(15) 14 9_565
Nd1 Bi5 Bi4 119.207(15) 6_554 9_565
Nd1 Bi5 Bi4 60.793(15) 5_554 9_565
Nd1 Bi5 Bi4 119.207(15) 13 9_565
Bi4 Bi5 Bi4 81.28(3) 9_665 9_565
Nd1 Bi5 Bi4 119.207(15) 14 1_655
Nd1 Bi5 Bi4 60.793(15) 6_554 1_655
Nd1 Bi5 Bi4 119.207(15) 5_554 1_655
Nd1 Bi5 Bi4 60.793(15) 13 1_655
Bi4 Bi5 Bi4 98.72(3) 9_665 1_655
Bi4 Bi5 Bi4 180.0 9_565 1_655
Nd1 Bi5 Bi4 119.208(15) 14 .
Nd1 Bi5 Bi4 60.792(15) 6_554 .
Nd1 Bi5 Bi4 119.208(15) 5_554 .
Nd1 Bi5 Bi4 60.792(15) 13 .
Bi4 Bi5 Bi4 180.0 9_665 .
Bi4 Bi5 Bi4 98.72(3) 9_565 .
Bi4 Bi5 Bi4 81.28(3) 1_655 .
Nd2 Bi6 Nd2 180.0 . 9
Nd2 Bi6 Bi2 60.893(13) . 13
Nd2 Bi6 Bi2 119.107(13) 9 13
Nd2 Bi6 Bi2 119.107(13) . 5_444
Nd2 Bi6 Bi2 60.893(14) 9 5_444
Bi2 Bi6 Bi2 180.00(3) 13 5_444
Nd2 Bi6 Bi2 60.893(13) . 14_445
Nd2 Bi6 Bi2 119.107(13) 9 14_445
Bi2 Bi6 Bi2 121.79(3) 13 14_445
Bi2 Bi6 Bi2 58.21(3) 5_444 14_445
Nd2 Bi6 Bi2 119.107(13) . 6_554
Nd2 Bi6 Bi2 60.893(13) 9 6_554
Bi2 Bi6 Bi2 58.21(3) 13 6_554
Bi2 Bi6 Bi2 121.79(3) 5_444 6_554
Bi2 Bi6 Bi2 180.00(3) 14_445 6_554
Nd2 Bi6 Bi2 60.893(13) . 14_545
Nd2 Bi6 Bi2 119.107(13) 9 14_545
Bi2 Bi6 Bi2 75.79(2) 13 14_545
Bi2 Bi6 Bi2 104.21(2) 5_444 14_545
Bi2 Bi6 Bi2 76.832(19) 14_445 14_545
Bi2 Bi6 Bi2 103.168(19) 6_554 14_545
Nd2 Bi6 Bi2 119.107(13) . 6_454
Nd2 Bi6 Bi2 60.893(13) 9 6_454
Bi2 Bi6 Bi2 104.21(2) 13 6_454
Bi2 Bi6 Bi2 75.79(2) 5_444 6_454
Bi2 Bi6 Bi2 103.168(19) 14_445 6_454
Bi2 Bi6 Bi2 76.832(19) 6_554 6_454
Bi2 Bi6 Bi2 180.00(3) 14_545 6_454
Nd2 Bi6 Bi2 119.107(13) . 5_544
Nd2 Bi6 Bi2 60.893(13) 9 5_544
Bi2 Bi6 Bi2 103.168(19) 13 5_544
Bi2 Bi6 Bi2 76.832(19) 5_444 5_544
Bi2 Bi6 Bi2 104.21(2) 14_445 5_544
Bi2 Bi6 Bi2 75.79(2) 6_554 5_544
Bi2 Bi6 Bi2 58.21(3) 14_545 5_544
Bi2 Bi6 Bi2 121.79(3) 6_454 5_544
Nd2 Bi6 Bi2 60.893(13) . 13_455
Nd2 Bi6 Bi2 119.107(13) 9 13_455
Bi2 Bi6 Bi2 76.832(19) 13 13_455
Bi2 Bi6 Bi2 103.168(19) 5_444 13_455
Bi2 Bi6 Bi2 75.79(2) 14_445 13_455
Bi2 Bi6 Bi2 104.21(2) 6_554 13_455
Bi2 Bi6 Bi2 121.79(3) 14_545 13_455
Bi2 Bi6 Bi2 58.21(3) 6_454 13_455
Bi2 Bi6 Bi2 180.00(2) 5_544 13_455
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Nd1 Bi3 3.2793(9) .
Nd1 Bi3 3.2793(9) 1_455
Nd1 Bi5 3.2886(11) 5_445
Nd1 Bi4 3.3341(9) 13
Nd1 Bi4 3.3341(9) 13_455
Nd1 Bi1 3.3628(10) 13
Nd1 Bi1 3.3628(10) 13_455
Nd1 Bi1 3.4595(14) .
Nd1 Bi2 3.4625(13) .
Nd2 Bi1 3.2517(9) .
Nd2 Bi1 3.2517(9) 2
Nd2 Bi3 3.2610(15) 1_455
Nd2 Bi3 3.2611(15) .
Nd2 Bi6 3.3014(16) .
Nd2 Bi2 3.4288(10) 14_445
Nd2 Bi2 3.4288(10) 13
Nd2 Bi2 3.4288(10) 13_455
Nd2 Bi2 3.4288(10) 14_545
Bi1 Bi1 3.1795(12) 13
Bi1 Bi1 3.1795(12) 13_455
Bi1 Bi2 3.1851(9) 13_455
Bi1 Bi2 3.1851(9) 13
Bi1 Nd1 3.3628(10) 13
Bi1 Nd1 3.3628(10) 13_455
Bi2 Bi1 3.1852(9) 13_455
Bi2 Bi1 3.1852(9) 13
Bi2 Bi2 3.3660(17) 10_556
Bi2 Nd2 3.4288(10) 13
Bi2 Nd2 3.4288(10) 13_455
Bi2 Bi6 3.4597(7) 5
Bi2 Bi6 3.4597(7) 5_455
Bi3 Nd2 3.2610(15) 1_655
Bi3 Nd1 3.2793(9) 1_655
Bi3 Nd1 3.2793(9) 2
Bi3 Nd1 3.2793(9) 2_655
Bi4 Bi5 3.3009(9) .
Bi4 Bi5 3.3009(9) 1_455
Bi4 Nd1 3.3341(9) 13
Bi4 Nd1 3.3341(9) 6_454
Bi4 Nd1 3.3341(9) 13_455
Bi4 Nd1 3.3341(9) 6_554
Bi5 Nd1 3.2886(11) 14
Bi5 Nd1 3.2886(11) 6_554
Bi5 Nd1 3.2886(11) 5_554
Bi5 Nd1 3.2886(11) 13
Bi5 Bi4 3.3008(9) 9_665
Bi5 Bi4 3.3008(9) 9_565
Bi5 Bi4 3.3008(9) 1_655
Bi6 Nd2 3.3014(16) 9
Bi6 Bi2 3.4598(7) 13
Bi6 Bi2 3.4598(7) 5_444
Bi6 Bi2 3.4598(7) 14_445
Bi6 Bi2 3.4598(7) 6_554
Bi6 Bi2 3.4598(7) 14_545
Bi6 Bi2 3.4598(7) 6_454
Bi6 Bi2 3.4598(7) 5_544
Bi6 Bi2 3.4598(7) 13_455
